Synthetic results of PIPPn. (Reproduced from Iwasaki et al., (2010)
There has been a great deal of interest in polyphosphoesters, which are biodegradable through hydrolysis and possibly through enzymatic digestion of phosphate linkages under physiological conditions (Renier et al., 1997). Biodegradable polyphosphoesters appear interesting for biological and pharmaceutical applications because of their biocompatibility and structural similarities to naturally occurring nucleic and teichoic acids. Recently, there have been interesting studies of polyphosphoesters used in biomedical applications (Wang et al., 2009). In particular, the advantages of polyphosphoesters for use in the field of tissue engineering as scaffolds and gene carriers was elucidated (Wan et al., 2001; Wang et al., 2002; Huang et al., 2004; Ren et al., 2010).
Figure 1 is a schematic representation of the contents of this chapter describing current research on polyphosphoesters. Although polyphosphoesters have a relatively long history, well-defined synthesis of the polymers has not been well explained. For use in medical applications such as drug delivery systems, understanding the synthetic process of polymers with narrow molecular weight distribution may be quite important to obtain reproducibility. The first part of this chapter discusses the controlled synthesis of polyphosphoesters.
In comparison with conventional biodegradable polymers, the molecular functionalization of polyphosphoesters is easier because varied cyclic phosphoesters, which work as monomers, can be obtained by a simple condensation reaction between alcohol and chloro cyclic phosphoesters. That is, theoretically, any alcohol can be introduced into polyphosphoesters. Here, a biodegradable macroinitiator and macrocrosslinker based on polyphosphoesters are described. They can be used as building blocks for preparing polymer blends and hydrogels.
We have also recently found that polyphosphoesters show thermoresponsivity in aqueous media. This polymer solution makes a lower critical solution temperature (LCST) type coacervate. The phenomenon is strongly influenced by the structure and molecular weight of the polymers and the solvent condition. The basic thermoresponsive properties of polyphosphoesters are summarized in this chapter. Enzyme-responsive polyphosphoesters are also introduced.
2. Synthesis of well-defied polyphosphoesters and incorporation of functional groups into polymers
A variety of synthetic routes for polyphosphoesters have been reported including ring-opening polymerization (ROP) (Libiszowski et al., 1978; Pretula et al., 1986), polycondensation (Richard et al, 1991), transesterfication (Pretula et al., 1999; Myrex et al., 2003), and enzymatic polymerization (Wen et al., 1998). Since the pioneering experiments by the Penczek group (Penczek & Klosinski, 1990), the ROP of cyclic phosphate has been studied for more than three decades and various polymers having a phosphoester backbone have been designed. The ROP of cyclic phosphoesters is the most common process used to obtain polyphosphoesters. This is because a variety of polyphosphoesters can be designed in comparison with conventional biodegradable polymers because cyclic phosphoesters are obtained as monomers from the condensation of alcohol and 2-chloro-2-oxo-1,3,2-dioxaphospholane (Katuiyhski et al., 1976).
2.1. Synthesis of polyphosphoesters using organocatalysts
For the ROP of cyclic phosphoesters, metallic compounds are commonly used as initiators or polymerization catalysts (Penczek et al., 1990; Libiszowski et al., 1978; Pretula et al., 1986; Xiao et al., 2006). Although the polymerization processes are very successful in producing polyphosphoesters, the metal compounds are environmentally sensitive and a lack of residual metal contaminants is required in biomedical applications. Recently, organocatalysts have been the focus of the modern synthetic processes of polyesters, polycarbonates, and silicones (Kamber et al., 2007). One of the most successful procedures for making biodegradable polymers is polymerization using guanidine and amidine bases, both in bulk and in solution. Nederberg and Hedrick prepared poly(trimethylene carbonate (TMC)) (PTMC) with the base catalysts in the presence of benzyl alcohol (Nederberg et al., 2007). Excellent controlled polymerization conditions were present with several catalysts, and PTMCs with relatively high molecular weight, narrow distribution, and high yield were obtained. We have recently recognized that organocatalysts have high potency for the ROP of cyclic phosphoesters (Iwasaki et al., 2010).
Poly(2-isopropoxy-2-oxo-1,3,2-dioxaphospholane) (PIPPn; n is degree of polymerization) was synthesized by ROP using an organocatalyst as an initiator in the presence of 2-hydroxyethyl-2’-bromoisobutyrate (HEBB) (Scheme 1). In the case of 1,8-diazabicyclo[5,4,0]undec-7-ene (DBU), polymerization was homogeneously performed in a solvent-free condition. In contrast, a small amount of toluene was used for dissolving 1,5,7-triazabicyclo[4,4,0]dec-5-ene (TBD) to make a homogeneous solution. The results of PIPP synthesis are summarized in Table 1. Twenty mmoles of IPP was first introduced into a polymerization tube under an argon gas atmosphere at 0°C, and then a given amount of HEBB was added to the tube. Finally, a given amount of organocatalyst was introduced. Polymerization was carried out at 0°C. The range of molecular weights was approximately 2.0 x 103 to 3.0 x 104 g/mol by gel-permeation chromatography (GPC) using a calibration curve based on linear polystyrene standards with chloroform as the mobile phase. In every case, the molecular weight distribution was lower than 1.10. Under each condition, the molecular weights of the synthetic polymers agreed with the theoretical values.
Figure 2 shows the number-averaged molecular weight (
2.2. Polyphosphoester macroinitiators
Atom transfer radical polymerization (ATRP) has great ability to control the molecular architecture of synthetic polymers and is an exceptionally robust method of producing block or graft copolymers (Matyjaszewski & Xia, 2001). However, the still limited design of biodegradable amphiphilic polymers has been performed via ATRP. Polyphosphoesters bearing 2-bromo-isobutyryl groups as novel biodegradable macroinitiators for ATRP were then synthesized and amphiphilic polymers with well–defined hydrophilic graft chains were prepared (Iwasaki & Akiyoshi, 2004).
A cyclic phosphoester bearing bromoisobutyrate, 2-(2-oxo,1,3,2-dioxaphospholoyloxy) ethyl-2’-bromoisobutyrate (OPBB), was obtained from the reaction of HEBB and 2-chloro-2-oxo-1,3,2-dioxaphosphorane (COP). Poly(IPP-co-OPBB) (PIxBry (Scheme 2); x:IPP (mol%), y: OPBB (mol%)) was synthesized by ring-opening polymerization using triisobutyl aluminum (TIBA) as an initiator. The chemical structure and synthetic results of the polyphosphoesters are shown in Scheme 2 and Table 2, respectively. Polymerization was homogeneously performed by a solvent-free reaction. As indicated in Table 2, the composition of each monomer unit could be controlled by the feed. The
ATRP of 2-methacryloyloxyethyl phosphorylcholine (MPC) from macroinitiator polyphosphoesters was carried out in an ethanol solution. Figure 3 shows the number of MPC units in a graft chain of PIBr2-g-PMPC and PIBr5-g-PMPC as determined by 1H NMR. The numbers were linearly increased with an increase in the duration of polymerization. The slope of the PIBr2-g-PMPC was much greater than that of PIBr5-g-PMPC. The rates of polymerization decreased with graft density.
|Mw x 10-4||No. of OPBB per PIBr molecule|
|In feed||In copolymer|
The transition point of the surface tension increased with an increase in the molecular weight and density of PMPC. Typical examples for the concentrations of PIBr3-g-PMPC71 The number after PMPC is degree of MPC polymerization in each graft chain.
The number after PMPC is degree of MPC polymerization in each graft chain.
Based on MALLS analysis for associative PIBr3-g-PMPC71, the molecular weight of the polymeric associate was 91.1 x 104. From the data in Figure 3, the molecular weight of PIBr3-g-PMPC71 can be estimated at 13.6 x 104. Thus, the association number of the PIBr3-g-PMPC71 was 6.7. For PIBr5-g-PMPC, the association number was 1.5, that is, it is almost a “unimer-micelle.” Figure 4 shows schematic representations of the polymeric associates of PIBr2-g-PMPC12 and PIBr5-g-PMPC115.
In an acidic medium, the loss of molecular weight of the graft copolymer was observed as being less; degradation remarkably occurred after 50 days of soaking. Under physiological pH conditions, the molecular weight of the PIBr-g-PMPC decreased from 15.6 x 104 (GPC data) to 12.7 x 104 after 50 days. Under a basic condition, the polyphosphoester degraded almost completely within 3 days. After soaking in pH11.0, the PIBr2-g-PMPC71 and PIBr5-g-PMPC115 polymers had molecular weights of 2.4 x 10-4 and 3.1 x 10-4 (
2.3. Polyphosphoester macrocrosslinkers
Biomaterials have an enormous impact on human health care. They are widely used in biomedical applications, including drug delivery devices and tissue engineering matrices (Lin et al., 2003). Specifically, hydrogels are included in the more recent development of biomaterials because they can absorb significant amounts of water and are as flexible as soft tissue, which minimizes their potential for irritating surrounding tissue. In order to obtain synthetic cellular matrices offering both biocompatibility and biodegradability, a novel porous biodegradable MPC polymer hydrogel crosslinked with polyphosphoesters was prepared with a gas-forming technique (Iwasaki et al., 2003; Iwasaki et al., 2004; Wachiralarpphaithoon et al., 2007).
|Potassium hydrogen carbonate size range (µm)||Swelling ratio|
(x 104 Pa)
The synthetic route of the macrocrosslinker, PIOP, was also synthesized using TIBA as an initiator (Scheme 4). The molecular weight of PIOP was 1.1 x 104 (
The synthetic conditions and characterizations of the hydrogels are summarized in Table 3. Figure 5 shows macroscopic pictures of the swollen hydrogels prepared in this study. The hydrogels (G1, G2, and G3) shown in picture a) were prepared without porogen salts. When the crosslinking density is low, the hydrogels have a highly stretched network, which was experimentally observed as a large transparent appearance. With an increase in the composition of PIOP, the size of the hydrogels decreased and the transparency became poor because of the close distance of the PIOP molecules. Picture b) shows porous hydrogels (G1A, G2A, and G3A) prepared with the largest porogen salts (
Alkaline phosphatase (ALP) is an important enzyme produced in bone and liver cells. It catalyzes the hydrolysis of phosphate groups from monophosphate ester substrates mostly found in an alkaline state with a pH of 9 (Coburn et al., 1998). Although Zhao and co-workers reported that synthetic polyphosphoesters and polyphosphoesters are enzymatically degradable (Zhao et al., 2003), the process was not described in detail. The concentration of ALP for the degradation study was adjusted to 72.5 and 220 U/L, which is the concentration in healthy adults and children, respectively (Takeshita et al., 2004; Rafan et al., 2000). Figure 6 is an enzymatic degradation profile of G1A hydrogels by changing the concentration of ALP. G1A took about 100 days to reach complete dissolution at pH 9.0. The degradation was accelerated with a higher concentration of ALP; G1A completely degraded after 60 days in 220 U/L of ALP. The degradation period was shortened with an increase in the concentration of the enzyme. The digestion of a hydrogel might be regulated by varying the density of cells secreting an enzyme in the hydrogel.
MC3T3-E1 is a clonal osteogenic cell line derived from neonatal mouse calvaria. The cells are well characterized and provide a homogeneous source of osteoblastic cells for study. They were encapsulated in various biomaterial networks and remained viable (Burdick et al., 2005). MC3T3-E1 cells express high levels of alkaline phosphatase and differentiate into osteoblasts that can form calcified bone tissue
Figure 7 shows the time-dependent concentration of the DNA produced from the MC3T3-E1 cells in porous hydrogels. The concentration increment of DNA corresponds to the proliferation of cells in a hydrogel. Under every sample condition, the amount of DNA significantly increased (p < 0.05) with increased cultivation time. After culture for 168 h, the amount of DNA collected was significantly higher from G3A (p = 0.036) in comparison to G1A. Therefore, the density of PIOP influenced cell proliferation. When the bFGF was incorporated into a hydrogel, the rate of cell proliferation relatively increased with an increase in the concentration of PIOP (p = 0.017 and p = 0.107 G1A vs. G3A after culture for 96 h and 168 h, respectively). While MPC polymer provides a suitable condition for maintaining cell viability, this polymer is not effective for inducing cell adhesion on the surface (Wachiralarpphaithoon et al., 2007). Polyphosphoester might induce cell adhesion and proliferation in a hydrogel. Wang and co-workers have recently reported that poly(ethylene glycol) (PEG) hydrogel having a phosphoester linkage promotes gene expression of bone-specific markers and secretion of alkaline phosphatase, osteocalcin, and osteonectin protein from marrow-derived mesenchymal stem cells (Wang et al., 2005).
3. Thermoresponsive polyphosphoesters
Thermoresponsive polymers are widely studied in both research and technology because of their versatility in many fields. Recent trends in the application of polymer materials are drug delivery (Kikuchi & Okano, 2002), separation of bioactive molecules (Kobayashi et al., 2003), and tissue engineering (Kikuchi & Okano, 2005).
Besides the stimuli-responsive nature, biodegradability and biocompatibility are important characteristics for polymeric materials used in biomedical fields. While the thermoresponsivity of some biodegradable polymers such as aliphatic polyester block copolymers or polypeptides was recently advanced (Fujiwara et al., 2001; Kim et al., 2004; Tachibana et al., 2003; Shimokuri et al., 2006), the molecular design and synthetic processes of thermoresponsive biodegradable polymers are still limited.
3.1. Thermoresponsivity of polyphosphoesters
In current research, thermoresponsive polyphosphoesters are now being synthesized with simple copolymerization of cyclic phosphoester compounds and their properties are being investigated (Iwasaki et al., 2007). Poly(IPP-co-EP) (PIxEy (Scheme 4); x:IPP (mol%), y: EP (mol%)) was synthesized by ring-opening polymerization using TIBA as an initiator. The range of weight-averaged molecular weights was 1.2 x 104 to 1.5 x 104 g/mol (GPC analysis).
Figure 8 shows the LCST-type phase separation of PI24E76 aqueous solution. From the optical microscopic image, it is clear that the polymer solution was separated at the liquid-liquid phase above the cloud point. This appears to be coacervation. After several hours, the turbid solution spontaneously separated into two phases. The cloud point could be controlled by the ratio of IPP and EP, that is, it decreased with an increase in the molar fraction of hydrophobic IPP.
Figure 9 shows the effect of the composition of the monomer unit on the LCST of the copolymers. The LCST of poly(EP) (PEP) was 38°C and it linearly decreased with an increase in the ratio of IPP. IPP is relatively hydrophobic; the homopolymer of IPP is not soluble in water above 5°C. Dehydration of the polymer then preferably occurred with the addition of the hydrophobic IPP unit. It is reported that the LCST of thermoresponsive polymers can be controlled by the ratio of the hydrophobic and hydrophilic units (Takei et al., 1993; Tachibana et al., 2003). Thermoresponsivity under physiological conditions is effective for drug delivery or tissue engineering applications (Okuyama et al., 1993; Nishida et al., 2004). The thermoresponsivity of polyphosphoesters can also be observed under physiological temperatures. Thus, the polymers are applicable in the biomedical field.
The effect of NaCl concentration on the cloud point on PEP and PI24E76 is shown in Figure 10. The cloud point of the polymer solution decreased with an increase in the concentration of NaCl in aqueous media. Under physiological conditions ([NaCl] = 100 mM), the cloud point of PEP and PI24E76 was 28 and 26°C, respectively. The solution property of nonionic polymer in water is sensitively influenced by the addition of salt because salt can alter polymer-water interaction (Foss et al., 1992).
Figure 11 shows the dependence of the cloud point of PI24E76 on polymer concentration in distilled water. The cloud point decreased with an increase in polymer concentration. Furthermore, the change in the transmittance of the polymer solution was more abrupt at a higher concentration. The effect of polymer concentration on phase separation temperature was also observed on poly(acryl amide) derivatives (Miyazaki & Kataoka, 1996). In their report, coacervate droplets could be condensed with centrifugation; the polymer concentration of the coacervate phase was much greater than that of the homogeneous solution.
|Temperature (°C)||Relaxation time (ms)|
(main chain CH2)
|Relaxation time (s)|
(side chain CH2)
|Relaxation time (s)|
(side chain CH3)
To understand the molecular phenomenon for creating coacervates, we measured
The relaxation times of the protons of associated trigger groups normally decrease because of a decrease in mobility (Hsu et al., 2005). However, the results did not show this. In the coacervate phase with enriched polymers, solvent remained above the cloud point. Then, the polymers might loosely associate and their mobility was not reduced with an increase in temperature. While the mobility of the polymers in the coacervate phase was clarified, further study will be needed to show the molecular mechanism of coacervation.
We demonstrated the separation of hydrophobic molecules with thermoresponsive polyphosphoesters from aqueous media. Nile Red was used as a model compound; its solubility in water is very low. Nile Red dissolved in acetone was added to Dulbecco’s phosphate buffered saline (PBS, calcium chloride- and magnesium chloride-free, Sigma). Polyphosphoester was then immediately introduced into the solution. Both PBS and that containing the polymer appear homogeneous before heating. When the solutions were incubated at 40°C, significant differences in solution behavior were observed, as shown in Figure 12. At 40°C, the polymer solution became turbid and then separated into two phases. Nile Red selectively condensed at the bottom layer, which contains the concentrated polymers. In contrast, the aggregation of Nile Red was observed in PBS at 40°C because the acetone evaporated and the Nile Red could not then disperse in the aqueous solution. After a decrease in temperature back to 4°C, the polymer solution appeared clear and homogeneous, but the aggregation of Nile Red remained in the PBS. The polyphosphoesters interact with hydrophobic Nile Red and help its dispersion. Furthermore, the precipitation of Nile Red was not observed even after the polymer solution was diluted 100 times with PBS. By using polyphosphoesters, we were able to improve the solubility of hydrophobic molecules in aqueous media and separate them with temperature increments.
Wang and co-workers also observed the thermoresponsivity of polyphosphoesters. They have synthesized well-defined block copolymers of poly(ethylene glycol) and polyphosphoester (Wang et al., 2009). Block copolymers can form core-shell type polymeric micelles in an aqueous medium with the effect of temperature caused by self-association of the polyphosphoester block. Although it is clear that polyphosphoester is the new candidate thermoresponsive polymer, its properties have only been partially evaluated. The effect of molecular weight on the cloud point of PIPPn (Scheme 1) has not been discussed. Figure 13 shows the dependence of the phase separation temperature of PIPP in phosphate buffered saline (PBS) on molecular weight.
The cloud point of the polymer solution decreases with an increase in the molecular weight of PIPP. The result indicates that the type of organocatalyst does not influence the phase separation temperature. The phase separation temperature of polyphosphoesters is influenced by the chemical structure of the side chains, the concentration, and the ion strength of the aqueous media. In our previous report, PIPP that was synthesized using TIBA as an initiator was not soluble in water even when the molecular weight was less than 1.0 x 104 (Iwasaki & Akiyoshi, 2004). An uncontrolled reaction might occur when a metallic catalyst was used. Wang reported that long-term polymerization of cyclic phosphoesters with Sn(Oct)2 makes some branch structures with high conversion rates (Xiao et al., 2006). In addition, some side reactions might occur in ring-opening polymerization of five-membered cyclic phosphoesters at high temperature (Liu et al., 2009). Furthermore, the molecular weight distribution of polyphosphoesters synthesized with an organocatalyst was significantly narrow compared with polymers that used metallic catalysts. The advantages of using organocatalysts can be observed on the synthesis of well-defined polymers with high conversion rates.
3.2. Polyphosphoester macroinitiators
Thermoresponsive polymers have great potential in bioscientific applications (Alarcon et al., 2005; Klouda et al., 2008). In particular, the selective delivery of drugs to target sites through hyperthermia could be performed (Chikoti et al., 2002). However, heat treatment might induce adverse effects on normal tissue and limitations remain in terms of selectivity. A polymer that can change its thermoresponsivity after contact with esterase has been synthesized. As shown in Scheme 5, polyphosphoesters bearing benzyl groups were synthesized. The synthetic results are listed in Table 5. The polymerization ability of BP and EP was similar. The 1H NMR spectra of the polymers at each reaction step are summarized in Figure 14. After treatment with Pd/C in formic acid, a signal caused by the aromatic group at around 7.2 ppm disappeared. Deprotection of benzyl groups from PEB was completely accomplished and PEH was obtained. Then, PEH reacted with acetoxymethyl bromide in the presence of ethyldiisopropylamine. The 1H NMR spectrum of PEHA clarified that the acetoxymethyl group was introduced at the deprotected position. No decrease in molecular weight was observed. No polymer degradation occurred during the introduction of the AM groups.
The enzymatic digestion of acetoxymethyl esters from PEHA was evaluated in contact with porcine liver esterase for a specific time. Figure 15 shows the time dependence of the relative fraction of the acetoxymethyl groups on the EP units. The data are represented as the mean from 4 samples. When the enzyme was treated with PEHA, the decrease in the fraction of AM groups was dramatic compared to that soaked in PBS for 24 h. The fraction then gradually decreased over time. Esterase activity might influence this data. Geurtsen and co-worker reported that the activity of porcine liver esterase decreased during the first 24 h to approximately 40% and then remained constant for up to 6 days (Geurtsen et al., 1999). Even in synthetic polymer systems, the effect of esterase has been observed. The AM groups spontaneously degraded in PBS. The degradation rate at the early stage was much slower than that of the esterase treatment.
|In feed||In copolymer|
Figure 16 shows the change in the number-averaged molecular weight (
The thermoresponsivity of PEHA before and after contact with protease is shown in Figure 17. The PEHA/PBS showed LCST-type liquid-liquid phase separation and the cloud point was 40°C. In both PBS and that with esterase, the temperature of the phase separation increased with an increase in incubation time. In particular, the PEHA treated with esterase for 24 h did not have a cloud point between 20 and 65°C. The degree of AM groups on the polymer influenced its thermoresponsivity. That is, the phase separation phenomena could be controlled by acetoxymethylation of the polyphosphoesters. In addition, PEH, the polymer before acetoxymethylation, did not show any LCST-type liquid-liquid phase separation (data not shown). The influence of the change in molecular weight of PEHA with esterase treatment should also be of concern. While the cloud point of PEHA synthesized in this study was not in physiological conditions (>40°C), it could be adjusted by introducing more hydrophobic units into the polymer as described in previous literature (Iwasaki et al., 2004). Because the block copolymers composed of polyphosphoesters and poly(ethylene glycol) form a micelle structure above phase separation temperature (Wang et al., 2009), PEHA will work as building blocks for making enzyme-responsive micelles.
The AM group is widely used for prodrugs and for fluorescence probes for cell imaging (Hecher et al., 2008; Takakusa et al., 2003). This group effectively induces cell membrane penetration and is rapidly cleaved intracellularly (Shultz et al., 1993; Yogo et al., 2004). Figure 18 is a fluorescence micrograph of HeLa cells in contact with Nile Red for 60 min with or without PEHA. The localization of Nile Red into the cells was improved by the presence of PEHA. At this concentration of PHEA, the polymer does not have a cloud point around 37°C. The solubilization capacity for hydrophobic molecules and the amphiphilic nature of the polymer might be improved by the cytoplasmic penetration of Nile Red. Although the mechanism of delivery of Nile Red into cells has not been fully clarified, the polyphosphoester bearing AM groups has the potential to induce penetration of hydrophobic drugs through the cell membrane.
To understand the interaction of PEHA and the cell membrane, we investigated the cytotoxicity of PEHA using Chinese hamster fibroblasts (V79), as described in a previous report (Iwasaki et al., 2004). There was no adverse effect of PEHA on cell viability when the PEHA concentration was below 0.01 g/dL (see supporting data). On the other hand, the cytotoxicity of PEHA was observed when the concentration was more than 0.1 g/dL. From the nature of this cytotoxicity test, it can be assumed that a high concentration of PEHA might damage the cell membrane. That is, that PHEA has an affinity for cell membrane.
This chapter described current studies of new methods of syntheses and the characteristics of polyphosphoesters. Polymerization with a narrow molecular weight distribution is important to obtain the reproducible properties of polymers. In addition, the functionalization of the end or side groups of the polymers results in producing various types of polymer materials. The robustness of polyphosphoesters as biomedical materials has been clarified during the past decade (Zhao et al., 1003; Wang et al., 2009). However, the molecular and material designs of polyphosphoesters for biomedical applications are still limited. Polyphosphoesters have been explored as biomimetic to nucleic and teichoic acids. The study of the biological activity of polyphosphoesters will prove to be interesting.
As one of the unique properties of polyphosphoesters, LCST-type liquid-liquid phase separation of polyphosphoesters in aqueous media was introduced with a difference in the structure of their side chains. The aqueous solution of the polymers bearing alkyl groups became turbid with increments in temperature. From microscopic observation, liquid-liquid phase separation was observed in the turbid solution. The cloud points of the polymer solutions were influenced by polymer concentration, copolymerization ratio, and NaCl concentration. In addition, the copolymer effectively improved the solubility of the hydrophobic molecules in an aqueous medium and enabled separation of the molecules from the solution with increments in temperature.
Furthermore, thermoresponsive polyphosphoesters bearing AM groups as side chains were demonstrated as enzyme-responsive polymers. The thermoresponsivity of polymers in aqueous solution depended on the concentration of AM units and their molecular weight. Cleavage of the AM units and degradation of the polymer chain were accelerated with esterase treatment. The solubility of hydrophobic molecules and localization of the molecules into living cells were also improved by the synthetic polymers. To use polyphosphoesters bearing AM groups as drug carriers, further molecular design to achieve self-assembly, stealth, and targeting characteristics will be needed. However, the newly designed structure is interesting as a basic motif for applications.
Some activities described in this chapter were supported by a Grant-in-Aid for Scientific Research on Innovative Areas "Molecular Soft-Interface Science" (#21106520) and Young Scientists (A) (#21680043) from the Ministry of Education, Culture, Sports, Science and Technology of Japan. The author is grateful to Dr. Shin-ichi Yusa (University of Hyogo), Ms. Etsuko Yamaguchi (Kansai University), and Mr. Takashi Kawakita (Kansai University) for their assistance in the synthesis and characterization of the polyphosphoesters.
- The number after PMPC is degree of MPC polymerization in each graft chain.